HAL Id: hal-01178579
Submitted on 24 May 2016
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Distributed under a Creative Commons Attribution - NonCommercial| 4.0 International
Initiation and propagation of a single pit on stainless
steel using a local probe technique
Stéphane Heurtault, Raphaël Robin, Fabien Rouillard, Vincent Vivier
To cite this version:
Stéphane Heurtault, Raphaël Robin, Fabien Rouillard, Vincent Vivier. Initiation and propagation of
a single pit on stainless steel using a local probe technique. Faraday Discussions, Royal Society of
Chemistry, 2015, 180, pp.267-282. �10.1039/c4fd00252k�. �hal-01178579v2�
Initiation and propagation of a single pit on
stainless steel using a local probe
St´ephane Heurtault,abRapha¨el Robin,aFabien Rouillard*a and Vincent Vivier*b
Received 8th December 2014, Accepted 2nd February 2015 DOI: 10.1039/c4fd00252k
Experiments about single pit initiation and propagation were performed on 316L stainless steel with the aim to determine the pitting corrosion behaviour for nuclear waste containers. The experimental setup permits to control the pit development at will and to create reproducible single pits in three dimensions. Radial and deep evolutions of a disc shaped pit were studied for propagation times of up to 10 hours. These evolutions were used to determine what limiting mechanism takes place during long-term pit propagation. Special attention has been paid to the chloride ion action on pitting. A minimum chloride concentration was found to be necessary in the bulk electrolyte to support pit propagation. The existence of a critical pit depth of 230 mm was also underlined.
Pitting corrosion is an important issue for the long-term behaviour of nuclear waste containers. Some containers may contain chloride-bearing polymers, which result in the production of chloride hydrogen gas by radiolysis. With the presence of humid zones formed on the inner 316L stainless steel container surface, the HCl gas completely dissolves and may form highly concentrated hydrochloric acid zones. Under these conditions, pits can initiate and propagate.
Pitting corrosion has been widely studied in the last decades on stainless steel,1,2but since it is a stochastic process, it remains diﬃcult to study
experi-mentally. Indeed adding an aggressive anion, such as chloride ion, to the elec-trolyte leads to the formation of several pits with diﬀerent stages of development on the material surface making any pitting analysis very diﬃcult. Many statistical studies have been performed to determine the pitting susceptibility of a
aCEA, DEN, DPC, SCCME, Laboratoire d'Etude de la Corrosion Non Aqueuse, F-91191 Gif-sur-Yvette, France. E-mail: email@example.com; Fax: +33-1-69081586; Tel: +33-1-69081614
bUniversit´e P. et M. Curie-CNRS, UMR8235, Laboratoire Interfaces et Syst`emes Electrochimiques, 4 place Jussieu, F-75005 Paris, France. E-mail: firstname.lastname@example.org; Fax: +33-1-44274074; Tel: +33-1-44274158 † Electronic supplementary information (ESI) available. See DOI: 10.1039/c4fd00252k
Cite this: Faraday Discuss., 2015, 180, 267
material.3–6 These studies focused on the frequencies of pit initiation and pit repassivation on a material surface on which several pits can evolve simulta-neously. The main results of this approach concern the probability to get a stable pit that cannot repassivate, the decrease of the pit generation rate with decreasing chloride concentration and the inuence of potential on the pitting rates. However, these statistical studies do not permit to highlight the driving forces of pitting corrosion and need to be complemented with mechanistic investigations. In addition, usual electrochemical measurements result in an average value on the electrode surface. Thus, to determine the mechanisms governing pitting corrosion from its initiation to the propagation or its repassivation, it is necessary to be able to work on a single pit.
Many researchers have attempted to create single pits. Diﬀerent methods have been used: an initial shape was given to the pit on the electrode surface using twin probe techniques,7 one-dimensional shielded wires,8 focus laser
illumination,9 or the electrode surface was partially covered to limit the
number of pits.10 These methods permit to study the early stage of pitting
corrosion. However, they have some disadvantages. First of all, the methods are not entirely reproducible from one experiment to the other. In some case these methods also damage the material surface. Also they cannot be used to study long-term pit growth. Depth evolution was studied in the literature with a lead-in-pencil electrode.11–14 It consisted of a wire, the diameter of which
varies from 10 to 50mm. This technique has the advantages to easily create single pits (such pits are called‘articial pits’) and to get simple pit geometry for further modelling. However, the lead-in-pencil electrode does not permit to have radius evolution. The radius evolution was independently investigated in the literature on aluminium,15,16 using a horizontal plate of a few
micrometers thick. This technique permitted to highlight the lateral evolution of the pit (but no work was performed on the depth evolution). Mixing the two last mentioned techniques with the introduction of a vertical foil in the lead-in-pencil technique, it was possible to study both lateral and vertical pit evolutions.17,18 However, due to the low thickness of the foil (from 25 to
50mm), which led to interactions between the pit and the resin, it was not possible to determine precise kinetic information about lateral evolution. In this article, an experimental setup allowing to locally inject chloride ions19–21 has been used to analyze the long-term development of a single pit in three dimensions.
It is generally admitted in the literature that long-term experiments are missing for pit propagation.1,10That is the scope of this article with the creation
and sustenance of a disc shaped single pit. Disc shaped pits are less studied than hemispherical pits despite the fact that they are more convenient for numerical modeling,22–24since they are obtained in a concentrated solution of chloride in which the number of pits is more important.
This paper aims at bringing new insight on the pit propagation description on 316L stainless steel. Aer the description of the experimental setup, the control of the initiation of a single pit will be detailed. Then, the propagation phase will be characterized and a particular attention will be paid to the description of both radial and deep evolutions. The last part of this article will focus on the pitting chemistry necessary to maintain the pit propagation.
Local electrochemical techniques have been widely used in corrosion investiga-tion.25,26The instrumentation used in this work was based on a scanning
elec-trochemical microscope (SECM), which has already been described elsewhere19–21
and in which the amperometric probe was replaced by a glass capillary (vide infra). The setup, sketched in Fig. 1, was composed of a lab-made potentiostat coupled with a low-noise-current-to-voltage converter (Femto DLPCA200, BFI Optilas) with an adjustable gain (103 to 1011 V A1) and a three-axis positioning system (VP-25XA, Newport) driven by a 100 nm spatial-resolution motion encoder (ESP300, Newport). The entire setup was controlled by a soware developed under Labview® environment. The glass microcapillary was used as a chloride ion dispenser to create a single pit on the stainless steel electrode. The top of the microcapillary was connected to a 300mL Terumo® syringe lled with a NaCl in a 0.5 M H2SO4solution. The eﬀect of the NaCl concentration has been studied by
varying its concentration in the syringe. A KD Scientic® syringe infusion pump was used to gradually release the solution at axed rate. The eﬀect of the releasing rate was also studied as a relevant parameter for the pit initiation/propagation. The lifetime of a microcapillary was extended by washing it with a water–ethanol mixture aer each experiment since the use of high concentration chloride solution may lead to crystal formation that obstruct its apex. All the experiments presented in this article were performed with the same glass microcapillary size with an inner diameter of 100mm and an outer diameter of 1000 mm. The precise positioning of the microcapillary was performed by measuring the electrolyte resistance between the substrate and the reference electrode.20This technique
was shown to be very sensitive to monitor the position of an insulating material in the close vicinity of a substrate.27 In a preliminary work, diﬀerent distances
between the microcapillary and the sample have been tested. If the distance was too large, several pits developed on the stainless steel surface. Thus, distances
Fig. 1 Electrochemical device developed for generating a single pit and studying its propagation.
between 10 to 20 mm have been chosen because corresponding to the larger distance at which a single pit was always observed.
2.2 Electrode preparation
The electrochemical cell was a three-electrode cell with a platinum grid acting as counter electrode, a mercury saturated sulphate electrode (MSE) as reference electrode (E¼ 650 mV/NHE) and a 316L stainless steel disk as working electrode. The nominal composition of the 316L stainless steel (in wt%) was obtained from EDAX analysis: 65.9% Fe, 18.5% Cr, 10.6% Ni, 2.4% Mo, 1.7% Mn and 0.9% Si. The stainless steel surface and the thickness of the sample were large enough to study the 3D evolution of the pit, allowing the progress in depth and radius of the single pit for a time longer than 10 hours to be investigated.
Surface preparation was important because it determined the passive lm nature, thickness, and its crystallization.28,29In this article, the same preparation
was always used to have a reproducible passivelm. The chosen surface prepa-ration was previously used in the literature by Hisamatsu et al.30and consisted in
several steps. First, the 316L stainless steel specimen was mechanically polished with 1200, 2400, and 4000 SiC paper, and then cleaned with a water and ethanol mixture in an ultrasonic bath for 10 min. Aer the polishing, the electrode was introduced in the electrolytic cell that will also be used for pitting corrosion experiments, and was then cathodically treated in 0.5 M H2SO4at0.9 V/MSE for
1 minute to reduce (at least partially) the native oxidelm. In the next step, the formation of the passivelm was achieved in the same electrolytic solution by performing a single potential sweep between 0.9 V/MSE and the working potential (i.e. the potential at which we wanted to initiate the pit) at a low scan rate (1 mV s1). Then, before releasing the chloride through the glass microcapillary, the working potential was held for 30 min to ensure that the passivelm is thick enough. In this work, all the experiments were performed at 0 V/MSE, but in a previous work21the eﬀect of the working potential on pitting was investigated.
The thickness of the passivelm at the end of the surface preparation was eval-uated by electrochemical impedance spectroscopy to be about 1 nm. This result is in good agreement with the work of Strehblow and Haupt29who measured the
passivelm thickness of Fe–15Cr in 0.5 M H2SO4from 1.1 nm at0.4 V/MSE to
1.9 nm at 0.4 V/MSE.
2.3 Physical characterization
Ex situ characterization of the pits was performed with a Leica Stereoscan 440 scanning electron microscope (SEM). This post-mortem observation allowed accurate measurements of the pit radius. The pit depth was measured using a diﬀerential focusing technique with an optical microscope equipped with a micrometric screw.
Results and discussion
3.1 Control of the pitting initiation
Fig. 2 shows 11 identical experiments performed independently. The solution injected with the microcapillary was 3 M NaCl with aow rate equal to 5.4 mL h1. The propagation time was varied between 3 and 40 minutes to allow ex situ pit
radius and depth characterizations at diﬀerent propagation times. The current– time records for the 11 identical experiments plotted in Fig. 2a were similar and included diﬀerent stages. First the initial time for the pitting in all of our experiments (i.e. t¼ 0 in Fig. 2) was dened as the time for which an increase in current due to pitting corrosion was monitored. The pit started to propagate aer the breakdown of the passive layer (just beneath the microcapillary and inde-pendent of the metal microstructure) due to the aggressiveness of chloride ions. Therst 10 to 15 minutes of the pit propagation were characterized by a sharp increase of current. Then the increases of the current slowed down. A similar current evolution between the 11 identical tests shows that the experimental setup permits to obtain reproducible single pits. Varying the working electrode disk diameter did not change the pitting reproducibility. Indeed, Fig. 3 shows that a similar current evolution was recorded for a 2 mm electrode diameter and a 4 mm electrode diameter. Aer 45 minutes of propagation, the pit radius and depth (determined with an optical microscope) were found to be 610mm and 147mm for a 2 mm in diameter working electrode, and 600 mm and 139 mm for a 4 mm electrode, respectively. It can be concluded that the electrode size did not modify the pitting evolution. However, the use of a smaller working electrode allowed us to investigate the early stage of the pitting since the background current (passive dissolution) is then minimized (data not shown), allowing a sharp evaluation of the onset of the current increase. The current evolution could be mainly explained by the increase of the pit radius while the pit depth seems to have a lower contribution, as shown in Fig. 2b. The initial sharp increase of current was linked with a huge increase of the pit radius while the pit depth did not exceed 25mm. This was ascribed to the large concentration of chloride used for the local pit initiation. This initial stage of the pit formation is linked with the inner and outer diameters of the microcapillary used to generate the single pit. Then the increases of the current and the pit radius slowed down together. In the literature such decreases of growth in current and pit radius were already found
Fig. 2 Current recorded (a) and mean geometric parameters of the pits (b) during the initiation of the pitting corrosion for 11 diﬀerent experiments at 0 V/MSE.
on iron under potentiostatic conditions and were explained by a salt lm precipitation.31
The inuence of the chloride amount brought by the microcapillary on the stainless steel disk was studied in two diﬀerent ways: (i) by varying the ow rate of the syringe driver, and (ii) by varying the NaCl concentration in the syringe. With both of these methods, similar results were obtained. Increasing the NaCl concentration in the syringe modied the pitting current as shown in Fig. 4. The initial current slope increased as did the step value of the current. The amount of chloride released by the microcapillary signicantly impacted the pit radius whereas the pit depth remained constant as shown in Fig. 5. A reproducible pit depth was found for experiments performed for 2 and 3 hours of propagation with variation of chloride introduction and the standard deviation was very low
Fig. 3 Current recorded during the single pit propagation experiments varying the diameter of the stainless steel electrode at 0 V/MSE.
Fig. 4 Current–time curves for three single pits after 1 hour propagation at 0 V/MSE with the chloride concentration as a parameter.
between each test (Table 1). The microscopy measurements showed that it was the increasing radius that could explain the current increase when the pit solution is more concentrated in chloride. Besides, increasing the amount of chloride brought by the microcapillary reduced the probability to have a pit cover of residual metal above the pit (Fig. 6). This shows that the whole stainless steel surface below the glass microcapillary dissolves when the solution is concen-trated enough in chloride. In addition, the small distance between the capillary and the steel electrode allowed for controlling the local environment in the close vicinity of the pit. Similar observations on the disappearance of the pit cover were reported in the literature but for increasing the potential32 and temperature33
instead of increasing the chloride concentration. In the following work, only pits without pit cover at the pit mouth were considered further. It should also be mentioned that the size of the microcapillary may play a non-negligible role on the pit initiation/propagation processes, especially the outer diameter of the glass part because the capillary and the steel substrate form a thin layer in which the electrolytic solution is conned.
3.2 Characterization of the pit propagation
The evolution of the pit geometry was investigated by performing 30 experiments for 11 diﬀerent pit propagation times between 45 minutes and 10 hours. Chloride ions were introduced in the electrochemical cell at a constantow rate of 5.4 mL h1using a 3 M NaCl and 0.5 M H2SO4solution. The ratio pit depth/pit radius at
Fig. 5 Inﬂuence of the chloride amount injected with the microcapillary on the geometric parameters of the pit after 2 hours of propagation at 0 V/MSE.
Table 1 Pit depth for two diﬀerent propagation times with the variation of the chloride amount brought to the system between each test
Propagation duration Number of performed experiments Mean depth (mm) Standard deviation for depth (mm) 2 hours 7 268 4 3 hours 10 360 8
the end of each experiment was calculated and plotted, shown in Fig. 7. For the whole tests, this ratio had approximately the same value of 0.4. As a consequence, the generated single pits are always disc shaped. It should also be mentioned that in the literature, most of the investigations are related to hemispherical pits.1,7,30,32,34Fig. 7 shows also the repartition of the 30 performed experiments
between the 11 propagation times. Reproducible pits were obtained for the propagation phase of up to 10 hours, as shown in Fig. 8a, for which the chro-noamperometry results between diﬀerent experiments overlap. During the propagation phase, the current increases slightly. In our experiments, aer 45 minutes of propagation, the current is proportional to t0.09. The measurement of the pit depth and pit diameter with an optical microscope and SEM allowed the determination of experimental laws for the evolution of the pit and the radius (Fig. 8b). For the radius the 11 experiments presented in the previous section for the initiation phase were also used because it was shown that the pit radius signicantly impacts the initiation phase whereas the pit depth evolution did not change between initiation and propagation. The following laws were found:
p ¼ 126 + 1.57|t 2700|0.54for t > 45 min (1)
r ¼ 250 + 26.36|t 180|0.34for t > 3 min (2)
Fig. 6 SEM images after 1 hour of propagation for the pits generated with 1.2 M NaCl + 0.5 M H2SO4(a), 2 M NaCl + 0.5 M H2SO4(b) and 3 M NaCl + 0.5 M H2SO4(c) in the syringe at
where p is the pit depth (expressed inmm), r the pit radius (in mm) and t the propagation time (in s).
In the experimental laws (1) and (2), the value of the diﬀerent parameters have a physical meaning. At 3 minutes (i.e. 180 s), we found a pit radius of 250mm. Aer 45 minutes (i.e. 2700 s), a pit depth of 126mm was found using eqn (1). These laws also revealed that the pit depth increases as a function of the square root of the time, whereas the radius grows as a function of t0.34. An increase in square root of
time is characteristic of a process limited by diﬀusion, suggesting that the pit bottom is rate determined by diﬀusion.
In the literature, for stainless steel Fe–18Cr–12Ni–2Mo–Ti in 0.5 M NaCl + 0.05 M H2SO4solution, Szklarska-Smialowska et al.35found under potentiostatic
conditions (at 0.860 V/NHE) that p t0.75and r t0.94. The diﬀerences with our results can be explained by the fact that they worked on a large electrode with many pits. As a consequence they obtained an average value on an unknown value of pits and at diﬀerent stages of the propagation process, whereas in this work, all the measurements are always performed on a single pit. In addition,uctuations of the current that preceded the formation of stable pits2due to the true passivity
breakdown36may have also vitiated the measurement.
A pit radius of 500mm, corresponding to the glass microcapillary radius, was obtained aer 15 minutes of propagation according to relation (2). For a pit radius greater than 500mm, the pit growth occurs under the stainless steel surface where the glass microcapillary is not present. In Fig. 9a, a pit growth under the stainless steel surface is noticeable at the periphery of the pit for a disc shaped pit aer more than 10 hours of propagation. This presence of a lacy cover is consistent with the potentiostatic investigations performed on 304 stainless steel foils in 1 M NaCl solution.17,18 Fig. 9b did not show any
crystallographic formation at the pit bottom, as it has been observed in the literature when the pit bottom potential is in the active state and when a salt lm is not present.37
Fig. 8 Current recorded (a) and mean geometric parameters of the pits (b) during the propagation of pitting corrosion for 30 diﬀerent experiments at 0 V/MSE.
Taking the derivative of eqn (1) and (2) allows the vertical and lateral pit growth rates to be expressed as:
dp dt¼ 0:86jt 2700j 0:46 for t . 45 min (3) dr dt¼ 8:98jt 180j 0:66 for t . 3 min (4)
For long-term propagation, the growth rate of the depth determined in relation (3) expressed inmm s1is lower than the growth rate of the radius written in relation (4) inmm s1. It is consistent with a disc shaped pit.
The Faraday law permits to link the electrochemical behavior with a mass loss proportional to the growth rates presented in relations (3) and (4). However, to use the Faraday law we need to know the oxidation number of species that dissolve. The hypothesis that there is no specic dissolution has been made and thus a mean oxidation number of 2.2 was used for 316L stainless steel. Fig. 10 validated the hypothesis of no specic dissolution. The pit volume corresponding to the metal dissolution was calculated by two diﬀerent methods. The direct route uses the Faraday law, which allowed for obtaining the volume of dissolution from the measured current. In the second approach, the calculation of volume was made from optical microscopy measurements and the hypothesis of a cylindrical pit was made. During the whole propagation time, both methods gave the same dissolution volume, suggesting that the use of the Faraday law is a valid hypothesis. The observation that the fraction of the dissolved elements in the solution aer pitting measured by ICP was equal to their fraction in the substrate conrms this result.20,21
From relations (3) and (4), using the Faraday law considering no specic dissolution and calculating theux, the local current densities on the pit walls and at pit bottom were determined to be:
Jpit bottom¼ rnF M dp dt for t . 45 min (5) Jpit walls¼ rnF M dr dt for t . 3 min (6) With Jlocal being the local current density, r being the 316L stainless steel
density (8 g cm3), n being the mean oxidation number involved in the corrosion
reaction (2.2), F being the Faraday constant (96 485 C mol1) and M being the 316L SS molar mass (56.1 g mol1).
These two relations are plotted in Fig. 11. The current density at the pit bottom decreases as a square root of time, revealing that the rate-limiting step at the pit bottom may be a diﬀusive process (see the ESI†). This might be the diﬀusion of metallic cations from the pit bottom to the pit mouth as defended several times in the literature.10,11,38,39 Another explanation was to consider that the limiting
diﬀusion is the transport of aggressive anions to the outside of the pit.31
Current density in a single pit had already been evaluated using articial pit electrodes. Isaacs11 determined the evolution of current density with time for
propagation times of up to 45 minutes for a 308 stainless steel immerged in 1 M NaCl. The initial value of current density was about 1.2 A m2, which is in good agreement with other works from the literature.37,40,41Then the current density
Fig. 10 Dissolution volume calculated by the Faraday law and by the optical measurements.
Fig. 11 Evolution of the current density on the pit walls and at the pit bottom for long-term pit propagation.
decreases in the square root of time to the value of 200 mA cm2aer 45 minutes of propagation. This value could be consistent with a current density of 125 mA cm2that we observed aer 1 hour of propagation. Newman13determined the
current density value for a longer propagation time, performing a single pit of 1 mm depth on a Fe–17Cr–11Ni–2.7Mo alloy using 4 M KCl solution. Aer reaching this depth, he changed the solution to 1 M KCl solution and then measured the current density at diﬀerent potentials. In our paper, using relation (1), a pit depth of 1 mm is obtained aer 34 hours of propagation. At 34 hours of propagation, a pit density of 10 mA cm2is calculated using relation (5). This value is also in good agreement with the one obtained by Newman for a lower overpotential.
3.3 Critical pitting chemistry
3.3.1 Corrosion product concentration at the pit bottom
The current density at the pit bottom was found to be lower than the current density on the pit walls (Fig. 11). This can be explained by the local chemistry at the pit bottom, which slows the corrosion rate but also permits to sustain the pit propagation. Using the Fickrst law, the concentration of metallic cations Men+at the pit bottom could be calculated from the following relationship:
Menþpit bottom¼ pr
With DMen+being the diﬀusion coeﬃcient of the metallic cations which was taken equal to 0.5 105cm2s1.11The bulk concentration of the metallic cations
(far from the pit) was also assumed to be zero.
During the single pit propagation, a constant concentration of 1.4 mol L1was found for the metallic cation concentration at the pit bottom (Fig. 12). Such a value corresponds to 30% of the saturation concentration of the solubility of FeCl2
(4.4 mol L1).42According to the literature,43,44the concentration of the corrosion
products within the pit must be maintained at about 60% for allowing the pit to propagate. However, a lower corrosion product concentration had already been reported in the literature for 304 stainless steel. Hisamatsu45 observed a pit
propagation with a corrosion product concentration of 1.8 M at the pit bottom (i.e. 40% of the saturation). Moreover, more complex iron salt with a lower solubility could have formed. This could be the case in our experiment with the formation of sulphate iron salts.
3.3.2 Critical bulk chloride concentration
The concentration of chloride required in the bulk electrolyte to maintain the pit propagation was determined. 20 reproducible single pits were created at 0 V/MSE releasing a solution of 3 M NaCl + 0.5 M H2SO4using the glass microcapillary with
a constantow rate of 5.4 mL h1. During the propagation, the bulk electrolyte was changed from a solution of 0.5 M H2SO4to a solution of 0.5 M H2SO4and variable
NaCl concentrations (C0) using peristaltic pumps working at constantow rates.
Aer 15 minutes, necessary to completely renew the bulk solution, the glass microcapillary was removed. Depending on the chloride concentration, C0, of the
bulk electrolyte, the pit propagation continued or stopped. As shown in Fig. 13, aer removing the microcapillary at 2 hours and 3 hours, it is noticeable that the pit still propagated for a bulk chloride concentration of 250 mM for both prop-agation times and that the pit repassivated for a lower bulk chloride concentra-tion of 235 mM.
The eﬀect of the bulk chloride concentration was studied as a function of pit propagation time and pit depth (Fig. 14). Each point in Fig. 14 represents one of the 20 performed experiments. Two zones can be clearly seen. A pit propagation zone may be dened for the bulk chloride concentration when it was high enough to sustain pit propagation. A pit repassivation zone exists when the bulk chloride concentration was no longer suﬃcient to maintain the propagation process. Between both zones, a critical chloride concentration may be dened. From
Fig. 12 Calculated concentration evolution at the pit bottom for long-term pit propagation.
Fig. 13 Chronoamperometries for 2 pitting experiments in which the microcapillary was removed after 2 hours (blue curves) and after 3 hours (red curves) to see if a critical chemistry exists in the bulk.
1 hour to 1 h 30 min of propagation, this critical concentration decreases. Then at 1 h 30 min of pit propagation, achieving a pit depth of 230mm, it reaches a step value between 235 mM and 250 mM. Additional experiments were performed at 235 mM and 250 mM of bulk chloride concentration to conrm the reproduc-ibility of the repassivation and propagation of the single pit aer 1 h 30 min of propagation. Conversely to iron or nickel,42stainless steel repassivates at a high
chloride concentration. The need of chloride ions to continue pit propagation was explained for the early stage of pit development by an increase of the saltlm volume during pit propagation as the pit surface grows. As the salt lm is composed of chloride ions, a supply of chloride ions is necessary to respond to the increased volume of the saltlm.42In addition, it was shown that the sulfate
concentration (data not shown) also plays a signicant role, since an increase in sulfate concentration is accompanied by a current decrease. For instance, in a 6 M sulfate solution (adding sulfate salt but maintaining a constant pH) the pitting current was 8 times smaller than in a 0.5 M solution. These observations are in good agreement with those reported by Pistorius and Burstein47on a 304 stainless
steel with the addition of SO42ion to a 1 M Clsolution. Indeed, these results
indicate the inuence of the chloride/sulphate ratio on the pitting behaviour and can be explained by a stronger adsorption of sulphate than chloride at the elec-trode interface.
The pitting corrosion of 316L stainless steel was investigated using an experi-mental setup that permits to create reproducible single pits. In the literature, pitting corrosion experiments usually focus on small hemispherical pits. Here, large disc shaped pits were analyzed with a propagation time of up to 10 hours. The experimental setup permitted to control at will the chloride ions brought into the pit solution. Experimental propagation laws for the geometrical parameters of
Fig. 14 Evolution of the critical chloride concentration necessary to continue the prop-agation of an opened pit with a radius of 800mm as a function of propagation time and pit depth.
the pit radius and depth were proposed. Calculations of local current densities were deducted to determine the limiting mechanism controlling the pit propa-gation. The pit growth at the pit bottom was limited by diﬀusion, probably due to the diﬀusion of the metallic cations from the bottom to the outside of the pit. A corrosion product concentration of 30% of the saturation was calculated at the pit bottom. This percentage, although lower than the one proposed in the literature, would be enough to prevent the pit repassivation. Experimentally, a minimum chloride concentration was determined in the bulk electrolyte to sustain the pit propagation. This concentration decreases with time until a critical pit depth of 230mm is reached. Then, the bulk electrolyte concentration has to be at least 245 mM NaCl to sustain the pit propagation on 316L austenitic stainless steel. Further investigations are under progress to investigate the inuence of the micro-capillary geometry and to determine geometrical laws for the pit radius and depth as a function of the chloride concentration.
The authors gratefully acknowledge AREVA NC for the funding of this project, and Françoise Pillier (UMR 8235) for the SEM observations.
1 Z. Szklarska-Smialowska, Electrochem. Soc., Proc., 2002, 13, 251. 2 J. Soltis, Corros. Sci., 2015, 90, 5.
3 T. Shibata and T. Takeyama, Corrosion, 1977, 33, 243.
4 D. E. Williams, C. Wescott and M. Fleischmann, Passivity of Metals and Semiconductors, ed. M. Froment, 1983, p. 217.
5 D. E. Williams, J. Stewart and P. H. Balkwill, Critical Factors in Localized Corrosion, ed. G. S. Frankel and R. C. Newman, 1992, p. 36.
6 D. E. Williams, J. Stewart and P. H. Balkwill, Corros. Sci., 1994, 36, 1213. 7 I. L. Rosenfeld and I. S. Danilov, Corros. Sci., 1967, 7, 129.
8 T. Beck, J. Electrochem. Soc., 1973, 120, 1317.
9 R. K. Ulrich and R. C. Alkire, Corros. Sci., 1983, 23, 1153. 10 R. C. Alkire and K. P. Wong, Corros. Sci., 1988, 28, 411. 11 H. S. Isaacs, J. Electrochem. Soc., 1973, 120, 1456.
12 R. C. Newman and H. S. Isaacs, Passivity of Metals and Semiconductors, ed. M. Froment, 1983, p. 269.
13 R. C. Newman, Corros. Sci., 1985, 25, 341.
14 N. J. Laycock and R. C. Newman, Mater. Sci. Forum, 1995, 192–194, 649. 15 G. S. Frankel, J. R. Scully and C. V. Jahnes, J. Electrochem. Soc., 1996, 143, 1834. 16 A. Sehgal, D. Lu and G. S. Frankel, J. Electrochem. Soc., 1998, 145, 2831. 17 P. Ernst and R. C. Newman, Corros. Sci., 2002, 44, 927.
18 S. M. Ghahari, D. P. Krouse, N. J. Laycock, T. Rayment, C. Padovani, T. Suter, R. Mokso, F. Marone, M. Stampanoni, M. Monir and A. J. Davenport, Corros. Eng., Sci. Technol., 2011, 46, 205.
19 N. Aouina, F. Balbaud-C´el´erier, F. Huet, S. Joiret, H. Perrot, F. Rouillard and V. Vivier, Electrochim. Acta, 2011, 56, 8589.
20 N. Aouina, F. Balbaud-C´el´erier, F. Huet, S. Joiret, H. Perrot, F. Rouillard and V. Vivier, Corros. Sci., 2012, 62, 1.
21 N. Aouina, F. Balbaud-C´el´erier, F. Huet, S. Joiret, H. Perrot, F. Rouillard and V. Vivier, Electrochim. Acta, 2013, 104, 274.
22 J. R. Galvele, J. Electrochem. Soc., 1976, 123, 464. 23 J. R. Galvele, Corros. Sci., 1981, 21, 551.
24 S. M. Gravano and J. R. Galvele, Corros. Sci., 1984, 24, 517.
25 L. Niu, Y. Yin, W. Guo, M. Lu, R. Qin and S. Chen, J. Mater. Sci., 2009, 44, 4511. 26 M. B. Jensen and D. E. Tallman, Electroanalytical Chemistry A Series of Advances,
ed. C. Bard and A. J. Zoski, 2011, vol. 24, p. 171.
27 H. Bouazaze, J. Fransaer, F. Huet, P. Rousseau and V. Vivier, Electrochim. Acta, 2010, 55, 1645.
28 A. J. Davenport, R. C. Newman and P. Ernst, Passivity of Metals and Semiconductors, ed. M. B. Ives, J. L. Luo and J. R. Rodda, 2001, Proceedings vol. 99–42, p. 65.
29 S. Haupt and H. H. Strehblow, Corros. Sci., 1994, 37, 43.
30 Y. Hisamatsu, T. Yoshii and Y. Matsumura, Localized Corrosion, ed. R. Staehle, NACE Houston, 1974, p. 427.
31 H. H. Strehblow and P. Marcus, Corrosion Mechanisms in Theory and Practise, ed. P. Marcus, 3rd edn, 2012, p. 349.
32 N. Sato, T. Nakagawa, K. Kudo and M. Sakashita, Localized Corrosion, ed. R. Staehle, NACE Houston, 1974, p. 447.
33 N. J. Laycock, M. H. Moayed and R. C. Newman, J. Electrochem. Soc., 1998, 145, 2622.
34 H. J. Engell and N. D. Stolica, Z. Phys. Chem., 1959, 20, 113.
35 Z. Szklarska-Smialowska and J. Mankowski, Corros. Sci., 1972, 12, 925. 36 G. T. Burstein and S. P. Mattin, Critical Factors in Localized Corrosion 2, ed. P.
M. Natishan, R. G. Kelly, G. S. Frankel and R. C. Newman, 1995, p. 1. 37 N. Sato, Corros. Sci., 1995, 37, 1947.
38 P. C. Pistorius and G. T. Burstein, Philos. Trans. R. Soc., A, 1992, 341, 531. 39 H. S. Isaacs and G. Kissel, J. Electrochem. Soc., 1972, 119, 1628.
40 W. Schwenk, Corrosion, 1964, 20, 129t.
41 V. M. Novokovsky and A. N. Sorokina, Proceedings Third International Congress Metallic Corrosion, MIR Publishers, Moscou, 1969, vol. 1, p. 159.
42 K. J. Vetter and H. H. Strehblow, Localized Corrosion, ed. R. Staehle, NACE Houston, 1974, p. 240.
43 G. T. Gaudet, W. T. Mo, T. A. Hatton, J. W. Tester, J. Tilly, H. S. Isaacs and R. C. Newman, AIChE J., 1986, 32, 949.
44 H. S. Isaacs, Corros. Sci., 1989, 29, 313.
45 Y. Hisamatsu, Passivity and its Breakdown on Iron and Iron Base Alloys, ed. R. W. Staehle and H. Okada, NACE Houston, 1976, p. 99.
46 K. J. Vetter, Electrochemical Kinetics, 1967, p. 214.